First Row Transition Metal(II) Thiocyanate Complexes, and Formation of 1-, 2-, and 3-Dimensional Extended Network Structures of M(NCS)2(Solvent)2 (M = Cr, Mn, Co) Composition
Endrit Shurdha; Curtis E. Moore; Arnold L. Rheingold; Saul H. Lapidus; Peter W. Stephens; Atta M. Arif; Joel S. Miller; Inorganic Chemistry 52 (2013) 10583–10594; doi:10.1021/ic401558f

data_4336063
_publ_contact_author_address
; 
Department of Chemistry
University of Utah
Salt Lake City
UT 84112-0850
USA
;
_publ_contact_author_email       jsmiller@chem.utah.edu
_publ_contact_author_name        'Joel S. Miller'
_publ_section_title
;
 First Row Transition Metal(II) Thiocyanate Complexes, and Formation of
 1-, 2-, and 3-Dimensional Extended Network Structures of
 M(NCS)2(Solvent)2 (M = Cr, Mn, Co) Composition
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              10583
_journal_page_last               10594
_journal_paper_doi               10.1021/ic401558f
_journal_volume                  52
_journal_year                    2013
_chemical_formula_moiety         'C6 N6 S6 Ni, C0.75 O0.25, 4(K)'
_chemical_formula_sum            'C6.75 K4 N6 O0.25 S6 V'
_chemical_formula_weight         578.101
_chemical_name_systematic
;
?
;
_space_group_IT_number           193
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      193
_symmetry_space_group_name_Hall  '-P 6c 2'
_symmetry_space_group_name_H-M   'P 63/m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   8.451111(78)
_cell_length_b                   8.451111
_cell_length_c                   9.16677(17)
_cell_measurement_temperature    295
_cell_volume                     566.989(12)
_computing_cell_refinement       TOPAS-Academic
_computing_data_collection       SPEC
_computing_data_reduction        TOPAS-Academic
_computing_structure_refinement  TOPAS-Academic
_computing_structure_solution    TOPAS-Academic
_diffrn_ambient_temperature      295
_diffrn_detector                 'NaI scintillation counter'
_diffrn_measurement_device_type  'Huber diffractometer'
_diffrn_radiation_monochromator  'Si(111) channel cut'
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.699974
_diffrn_source                   synchrotron
_pd_block_diffractogram_id       ES-2-26
_pd_instr_location
;
X16C, National Synchrotron Light Source, Brookhaven National Laboratory
;
_pd_meas_2theta_range_inc        0.005
_pd_meas_2theta_range_max        45.0
_pd_meas_2theta_range_min        5.0
_pd_meas_number_of_points        8001
_pd_meas_scan_method             step
_pd_proc_2theta_range_inc        0.005
_pd_proc_2theta_range_max        45.0
_pd_proc_2theta_range_min        5.0
_pd_proc_ls_background_function
;
9 Pearson-Voight peaks and Chebyshev polynomial with 79 coefficients
;
_pd_proc_ls_pref_orient_corr
;
none
;
_pd_proc_ls_profile_function
;
Simple_Axial_model function with Rp=9999,Rs=330 in TOPAS-Academic
;
_pd_proc_ls_prof_R_factor        0.04543
_pd_proc_ls_prof_wR_expected     0.0165
_pd_proc_ls_prof_wR_factor       0.05857
_pd_proc_wavelength              0.699974
_pd_spec_mounting
;
capillary
;
_pd_spec_mount_mode              transmission
_pd_spec_shape                   cylinder
_refine_ls_goodness_of_fit_all   3.549
_refine_ls_number_parameters     79
_refine_ls_weighting_details     1/(sigma*sigma)
_refine_ls_weighting_scheme      sigma
_cod_data_source_file            ic401558f_si_002_10.cif
_cod_data_source_block           ES-2-26
_cod_original_cell_volume        566.989(18)
_cod_original_formula_sum        'C6.75 K4 N6 O0.25 S6 V1'
_cod_database_code               4336063